LMucko/crystallography-open-database huggingface dataset:
Crystal structures of eight mono-methyl alkanes (C~26~–C~32~) <i>via</i> single-crystal and powder diffraction and DFT-D optimization
Brooks, Lee; Brunelli, Michela; Pattison, Philip; Jones, Graeme R.; Fitch, Andrew; IUCrJ 2 (2015) 490–497; doi:10.1107/S2052252515010271

data_1542830
_publ_section_title
;
 Crystal structures of eight mono-methyl alkanes (C~26~--C~32~) <i>via</i>
 single-crystal and powder diffraction and DFT-D optimization
;
_journal_issue                   5
_journal_name_full               IUCrJ
_journal_page_first              490
_journal_page_last               497
_journal_paper_doi               10.1107/S2052252515010271
_journal_volume                  2
_journal_year                    2015
_chemical_absolute_configuration S
_chemical_formula_moiety         'C26 H54'
_chemical_formula_sum            'C26 H54'
_chemical_formula_weight         366.71
_chemical_name_systematic
;
(<i>S</i>)-9-methylpentacosane
;
_space_group_IT_number           4
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.6247(15)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   21.44393(75)
_cell_length_b                   4.937406(76)
_cell_length_c                   12.34557(40)
_cell_measurement_temperature    80
_cell_volume                     1258.81(6)
_diffrn_ambient_temperature      80
_diffrn_radiation_monochromator  'Si 111'
_diffrn_radiation_type           'Synchrotron ID31 at ESRF'
_diffrn_radiation_wavelength     0.80025
_exptl_crystal_colour            white
_exptl_crystal_density_diffrn    0.967
_exptl_crystal_description       powder
_publcif_datablock.id            {9fb0a388-eec5-44ab-b47c-7077ee28c2b9}
_cod_data_source_file            lc5062.cif
_cod_data_source_block           9MeC25H51
_cod_original_cell_volume        1258.815(64)
_cod_original_sg_symbol_H-M      P21
_cod_database_code               1542830
Crystal structures of eight mono-methyl alkanes (C~26~–C~32~) <i>via</i> single-crystal and powder diffraction and DFT-D optimization
Brooks, Lee; Brunelli, Michela; Pattison, Philip; Jones, Graeme R.; Fitch, Andrew; IUCrJ 2 (2015) 490–497; doi:10.1107/S2052252515010271

data_1542831
_publ_section_title
;
 Crystal structures of eight mono-methyl alkanes (C~26~--C~32~) <i>via</i>
 single-crystal and powder diffraction and DFT-D optimization
;
_journal_issue                   5
_journal_name_full               IUCrJ
_journal_page_first              490
_journal_page_last               497
_journal_paper_doi               10.1107/S2052252515010271
_journal_volume                  2
_journal_year                    2015
_chemical_absolute_configuration S
_chemical_formula_moiety         'C28 H58'
_chemical_formula_sum            'C28 H58'
_chemical_formula_weight         394.76
_chemical_name_systematic
;
(<i>S</i>)-9-methylheptacosane
;
_space_group_IT_number           4
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_cell_angle_alpha                90
_cell_angle_beta                 109.2946(24)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   23.4884(13)
_cell_length_b                   4.93921(10)
_cell_length_c                   12.33521(59)
_cell_measurement_temperature    100
_cell_volume                     1350.68(10)
_diffrn_ambient_temperature      100
_diffrn_radiation_monochromator  'Si 111'
_diffrn_radiation_type           'Synchrotron ID31 at ESRF'
_diffrn_radiation_wavelength     0.80105
_exptl_crystal_colour            white
_exptl_crystal_density_diffrn    0.971
_exptl_crystal_description       powder
_publcif_datablock.id            {8ccf4750-5d9f-4eaa-bdff-4c8997fa7b74}
_cod_data_source_file            lc5062.cif
_cod_data_source_block           9MeC27H55
_cod_original_sg_symbol_H-M      P21
_cod_database_code               1542831
Crystal structures of eight mono-methyl alkanes (C~26~–C~32~) <i>via</i> single-crystal and powder diffraction and DFT-D optimization
Brooks, Lee; Brunelli, Michela; Pattison, Philip; Jones, Graeme R.; Fitch, Andrew; IUCrJ 2 (2015) 490–497; doi:10.1107/S2052252515010271

data_1542832
_publ_section_title
;
 Crystal structures of eight mono-methyl alkanes (C~26~--C~32~) <i>via</i>
 single-crystal and powder diffraction and DFT-D optimization
;
_journal_issue                   5
_journal_name_full               IUCrJ
_journal_page_first              490
_journal_page_last               497
_journal_paper_doi               10.1107/S2052252515010271
_journal_volume                  2
_journal_year                    2015
_chemical_absolute_configuration S
_chemical_formula_moiety         'C30 H62'
_chemical_formula_sum            'C30 H62'
_chemical_formula_weight         422.81
_chemical_name_systematic
;
(<i>S</i>)-9-methylnonacosane
;
_space_group_IT_number           4
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_cell_angle_alpha                90
_cell_angle_beta                 112.4482(40)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   25.6203(18)
_cell_length_b                   4.93638(18)
_cell_length_c                   12.32668(91)
_cell_measurement_temperature    100
_cell_volume                     1440.84(16)
_diffrn_ambient_temperature      100
_diffrn_radiation_monochromator  'Si 111'
_diffrn_radiation_type           'Synchrotron ID31 at ESRF'
_diffrn_radiation_wavelength     0.80105
_exptl_crystal_colour            white
_exptl_crystal_density_diffrn    0.975
_exptl_crystal_description       powder
_publcif_datablock.id            {7fd36ea1-8562-4ed7-9ead-8489a4b58ee9}
_cod_data_source_file            lc5062.cif
_cod_data_source_block           9MeC29H59
_cod_original_sg_symbol_H-M      P21
_cod_database_code               1542832
Crystal structures of eight mono-methyl alkanes (C~26~–C~32~) <i>via</i> single-crystal and powder diffraction and DFT-D optimization
Brooks, Lee; Brunelli, Michela; Pattison, Philip; Jones, Graeme R.; Fitch, Andrew; IUCrJ 2 (2015) 490–497; doi:10.1107/S2052252515010271

data_1542833
_publ_section_title
;
 Crystal structures of eight mono-methyl alkanes (C~26~--C~32~) <i>via</i>
 single-crystal and powder diffraction and DFT-D optimization
;
_journal_issue                   5
_journal_name_full               IUCrJ
_journal_page_first              490
_journal_page_last               497
_journal_paper_doi               10.1107/S2052252515010271
_journal_volume                  2
_journal_year                    2015
_chemical_absolute_configuration S
_chemical_formula_moiety         'C32 H66'
_chemical_formula_sum            'C32 H66'
_chemical_formula_weight         450.87
_chemical_name_systematic
;
(<i>S</i>)-9-methylhentriacontane
;
_space_group_IT_number           4
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.67967(77)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   27.78145(44)
_cell_length_b                   4.933812(40)
_cell_length_c                   12.38987(21)
_cell_measurement_temperature    100
_cell_volume                     1530.52(4)
_diffrn_ambient_temperature      100
_diffrn_radiation_monochromator  'Si 111'
_diffrn_radiation_type           'Synchrotron ID31 at ESRF'
_diffrn_radiation_wavelength     0.80105
_exptl_crystal_colour            white
_exptl_crystal_density_diffrn    0.978
_exptl_crystal_description       powder
_publcif_datablock.id            {9d67a276-decb-4a58-bd35-697e72e737bb}
_cod_data_source_file            lc5062.cif
_cod_data_source_block           9MeC31H63
_cod_original_cell_volume        1530.525(39)
_cod_original_sg_symbol_H-M      P21
_cod_database_code               1542833
Crystal structures of eight mono-methyl alkanes (C~26~–C~32~) <i>via</i> single-crystal and powder diffraction and DFT-D optimization
Brooks, Lee; Brunelli, Michela; Pattison, Philip; Jones, Graeme R.; Fitch, Andrew; IUCrJ 2 (2015) 490–497; doi:10.1107/S2052252515010271

data_1542834
_publ_section_title
;
 Crystal structures of eight mono-methyl alkanes (C~26~--C~32~) <i>via</i>
 single-crystal and powder diffraction and DFT-D optimization
;
_journal_issue                   5
_journal_name_full               IUCrJ
_journal_page_first              490
_journal_page_last               497
_journal_paper_doi               10.1107/S2052252515010271
_journal_volume                  2
_journal_year                    2015
_chemical_absolute_configuration S
_chemical_formula_moiety         'C30 H62'
_chemical_formula_sum            'C30 H62'
_chemical_formula_weight         422.81
_chemical_name_systematic
;
(<i>S</i>)-7-methylnonacosane
;
_space_group_IT_number           4
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.40592(59)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   28.09291(37)
_cell_length_b                   4.932501(29)
_cell_length_c                   10.36893(12)
_cell_measurement_temperature    100
_cell_volume                     1436.77(3)
_diffrn_ambient_temperature      100
_diffrn_radiation_monochromator  'Si 111'
_diffrn_radiation_type           'Synchrotron ID31 at ESRF'
_diffrn_radiation_wavelength     0.80105
_exptl_crystal_colour            white
_exptl_crystal_density_diffrn    0.977
_exptl_crystal_description       powder
_publcif_datablock.id            {159b0e8b-ad10-4793-ada3-0e4064d7c8d1}
_publcif_info_exptl_table_max_cols 4
_publcif_info_exptl_table_use_headnotes n
_cod_data_source_file            lc5062.cif
_cod_data_source_block           7MeC29H59
_cod_original_cell_volume        1436.769(26)
_cod_original_sg_symbol_H-M      P21
_cod_database_code               1542834
Structure and reorientational dynamics of 1-F-adamantane.
Ben Hassine, B.; Negrier, Ph; Romanini, M.; Barrio, M.; Macovez, R.; Kallel, A.; Mondieig, D.; Tamarit, J. Ll; Physical chemistry chemical physics : PCCP 18 (2016) 10924–10930; doi:10.1039/c6cp01144f

data_7224637
_publ_section_title
;
 Structure and reorientational dynamics of 1-F-adamantane.
;
_journal_issue                   16
_journal_name_full               'Physical chemistry chemical physics : PCCP'
_journal_page_first              10924
_journal_page_last               10930
_journal_paper_doi               10.1039/c6cp01144f
_journal_volume                  18
_journal_year                    2016
_chemical_formula_sum            'C10 H15 F'
_chemical_formula_weight         154.22
_space_group_IT_number           225
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_audit_creation_date             2015-10-21
_audit_creation_method           'Materials Studio'
_cell_angle_alpha                90.0000
_cell_angle_beta                 90.0000
_cell_angle_gamma                90.0000
_cell_formula_units_Z            4
_cell_length_a                   9.5522(4)
_cell_length_b                   9.5522(4)
_cell_length_c                   9.5522(4)
_cell_measurement_temperature    295(1)
_cell_measurement_theta_max      45.0
_cell_measurement_theta_min      7.5
_cell_volume                     871.59(6)
_diffrn_ambient_temperature      295(1)
_diffrn_measurement_device_type  'Inel CPS120'
_diffrn_radiation_monochromator  'curved quartz'
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           CuK\a~1~
_diffrn_radiation_wavelength     1.540562
_exptl_crystal_colour            White
_exptl_crystal_density_diffrn    1.175
_exptl_crystal_description       'Powder Sample'
_cod_data_source_file            c6cp01144f2.cif
_cod_data_source_block           'global_AdaFluoro295K'
_cod_depositor_comments
'Adding full bibliography for 7224637--7224638.cif.'
_cod_original_cell_volume        871.59(11)
_cod_original_sg_symbol_H-M      'F M -3 M'
_cod_database_code               7224637
Structure and reorientational dynamics of 1-F-adamantane.
Ben Hassine, B.; Negrier, Ph; Romanini, M.; Barrio, M.; Macovez, R.; Kallel, A.; Mondieig, D.; Tamarit, J. Ll; Physical chemistry chemical physics : PCCP 18 (2016) 10924–10930; doi:10.1039/c6cp01144f

data_7224638
_publ_section_title
;
 Structure and reorientational dynamics of 1-F-adamantane.
;
_journal_issue                   16
_journal_name_full               'Physical chemistry chemical physics : PCCP'
_journal_page_first              10924
_journal_page_last               10930
_journal_paper_doi               10.1039/c6cp01144f
_journal_volume                  18
_journal_year                    2016
_chemical_formula_sum            'C10 H15 F'
_chemical_formula_weight         154.22
_space_group_IT_number           114
_symmetry_cell_setting           tetragonal
_symmetry_Int_Tables_number      114
_symmetry_space_group_name_Hall  'P -4 2n'
_symmetry_space_group_name_H-M   'P -4 21 c'
_audit_creation_date             2015-10-21
_audit_creation_method           'Materials Studio'
_cell_angle_alpha                90.0000
_cell_angle_beta                 90.0000
_cell_angle_gamma                90.0000
_cell_formula_units_Z            2
_cell_length_a                   6.7776(3)
_cell_length_b                   6.7776(3)
_cell_length_c                   8.8235(5)
_cell_measurement_temperature    100(1)
_cell_measurement_theta_max      52.5
_cell_measurement_theta_min      7.5
_cell_volume                     405.32(3)
_diffrn_ambient_temperature      100(1)
_diffrn_measurement_device_type  'Inel CPS120'
_diffrn_radiation_monochromator  'curved quartz'
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           CuK\a~1~
_diffrn_radiation_wavelength     1.540562
_exptl_crystal_colour            White
_exptl_crystal_density_diffrn    1.264
_exptl_crystal_description       'Powder Sample'
_cod_data_source_file            c6cp01144f1.cif
_cod_data_source_block           'global_AdaFluoro100K'
_cod_depositor_comments
'Adding full bibliography for 7224637--7224638.cif.'
_cod_original_cell_volume        405.32(4)
_cod_original_sg_symbol_H-M      P-421C
_cod_database_code               7224638
Spin-glass Magnetism in RFeTi2O7 (R=Lu and Tb) Compounds
T.V. Drokina; G.A. Petrakovskii; M.S. Molokeev; A. Arauzo; J. Bartolome; Physics Procedia 75 (2014) 580–588; doi:10.1016/j.phpro.2015.12.074

data_1542916
_publ_section_title
;
 Spin-glass Magnetism in RFeTi2O7 (R=Lu and Tb) Compounds
;
_journal_issue                   0
_journal_name_full               'Physics Procedia'
_journal_page_first              580
_journal_page_last               588
_journal_paper_doi               10.1016/j.phpro.2015.12.074
_journal_volume                  75
_journal_year                    2014
_chemical_formula_moiety         'Fe7.34 O56 Tb8 Ti16.66'
_chemical_formula_sum            'Fe7.34 O56 Tb8 Ti16.66'
_chemical_formula_weight         3374.86
_space_group_IT_number           60
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2b 2ac'
_symmetry_space_group_name_H-M   'P c n b'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   9.85680(13)
_cell_length_b                   13.59424(18)
_cell_length_c                   7.37880(11)
_cell_measurement_temperature    300
_cell_volume                     988.73(2)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    117.827
_exptl_crystal_density_diffrn    5.6530(13)
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.016
_pd_meas_2theta_range_max        139.987
_pd_meas_2theta_range_min        5
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
no correction
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        1.068
_pd_proc_ls_prof_wR_expected     0.707
_pd_proc_ls_prof_wR_factor       1.153
_pd_proc_number_of_points        8436.6875
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   1.631
_refine_ls_R_I_factor            0.52
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            TbFeTi2O7.cif
_cod_data_source_block           a
_cod_original_cell_volume        988.728(23)
_cod_original_sg_symbol_Hall
;
-P 2b 2ac
;
_cod_original_sg_symbol_H-M      Pcnb
_cod_original_formula_sum
;
Fe7.34 O56 Tb8 Ti16.66
;
_cod_database_code               1542916
_cod_database_fobs_code          1542916
Pressure-stimulated synthesis and luminescence properties of microcrystalline (Lu,Y)3Al5O12:Ce3+ garnet phosphors
V.V. Atuchin; N.F. Beisel; E.N. Galashov; E.M. Mandrik; M.S. Molokeev; A.P. Yelisseyev; A.A. Yusuf; Zhiguo Xia; ACS Applied Materials & Interfaces 7 (2015) 26235–26243; doi:10.1021/acsami.5b08411

data_4513851
_publ_section_title
;
 Pressure-stimulated synthesis and luminescence properties of
 microcrystalline (Lu,Y)3Al5O12:Ce3+ garnet phosphors
;
_journal_issue                   47
_journal_name_full               'ACS Applied Materials & Interfaces'
_journal_page_first              26235
_journal_page_last               26243
_journal_paper_doi               10.1021/acsami.5b08411
_journal_volume                  7
_journal_year                    2015
_chemical_formula_moiety         'Al40 Ce0.07 Lu23.83 O96 Y0.07'
_chemical_formula_sum            'Al40 Ce0.07 Lu23.83 O96 Y0.07'
_chemical_formula_weight         6801.58
_space_group_IT_number           230
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-I 4bd 2c 3'
_symmetry_space_group_name_H-M   'I a -3 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   11.917055(36)
_cell_length_b                   11.917055(36)
_cell_length_c                   11.917055(36)
_cell_measurement_temperature    300
_cell_volume                     1692.415(9)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    70.764
_exptl_crystal_density_diffrn    6.676681
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.0160352
_pd_meas_2theta_range_max        140.000349
_pd_meas_2theta_range_min        5
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
no preferred orientation effect
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        6.514
_pd_proc_ls_prof_wR_expected     6.562
_pd_proc_ls_prof_wR_factor       8.229
_pd_proc_number_of_points        8419
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   1.254
_refine_ls_R_I_factor            3.21
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            Lu2p98Ce0p01Y0p01Al5O12.cif
_cod_data_source_block           a
_cod_original_cell_volume        1692.415(15)
_cod_original_sg_symbol_Hall
;
-I 4bd 2c 3
;
_cod_original_sg_symbol_H-M      Ia-3d
_cod_original_formula_sum
;
Al40 Ce0.07 Lu23.83 O96 Y0.07
;
_cod_database_code               4513851
_cod_database_fobs_code          4513851
Pressure-stimulated synthesis and luminescence properties of microcrystalline (Lu,Y)3Al5O12:Ce3+ garnet phosphors
V.V. Atuchin; N.F. Beisel; E.N. Galashov; E.M. Mandrik; M.S. Molokeev; A.P. Yelisseyev; A.A. Yusuf; Zhiguo Xia; ACS Applied Materials & Interfaces 7 (2015) 26235–26243; doi:10.1021/acsami.5b08411

data_4513852
_publ_section_title
;
 Pressure-stimulated synthesis and luminescence properties of
 microcrystalline (Lu,Y)3Al5O12:Ce3+ garnet phosphors
;
_journal_issue                   47
_journal_name_full               'ACS Applied Materials & Interfaces'
_journal_page_first              26235
_journal_page_last               26243
_journal_paper_doi               10.1021/acsami.5b08411
_journal_volume                  7
_journal_year                    2015
_chemical_formula_moiety         'Al10 Ce0.02 O24 Y5.98'
_chemical_formula_sum            'Al10 Ce0.02 O24 Y5.98'
_chemical_formula_weight         1188.18
_space_group_IT_number           230
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-I 4bd 2c 3'
_symmetry_space_group_name_H-M   'I a -3 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.012905(29)
_cell_length_b                   12.012905(29)
_cell_length_c                   12.012905(29)
_cell_measurement_temperature    300
_cell_volume                     1733.581(7)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    32.452
_exptl_crystal_density_diffrn    4.552724
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.0160352
_pd_meas_2theta_range_max        140.000349
_pd_meas_2theta_range_min        5
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
no preferred orientation
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        9.250
_pd_proc_ls_prof_wR_expected     8.743
_pd_proc_ls_prof_wR_factor       11.726
_pd_proc_number_of_points        8419
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   1.341
_refine_ls_R_I_factor            4.14
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            Y2p99Ce0p01Al5O12.cif
_cod_data_source_block           a
_cod_original_cell_volume        1733.581(12)
_cod_original_sg_symbol_Hall
;
-I 4bd 2c 3
;
_cod_original_sg_symbol_H-M      Ia-3d
_cod_original_formula_sum
;
Al10 Ce0.02 O24 Y5.98
;
_cod_database_code               4513852
_cod_database_fobs_code          4513852